SLURRY PHASE IRON CATALYSTS FOR INDIRECT COAL LIQUEFACTION
Semi-Annual Technical Report
Reporting Period: July 4, 1996 - January 5, 1997
Author: Abhaya K. Datye
Report Issue Date: February, 1997
University of New MexicoCenter for Microengineered Materials
Albuquerque, NM 87131
This report was prepared as an account of work sponsored by an agency of the United States Gov-ernment. Neither the United States Government nor any agency thereof, nor any of their employees,makes any warranty, express or implied, or assumes any legal liability or responsibility for theaccuracy, completeness, or usefulness of any information, apparatus, product or process disclosed, orrepresents that its use would not infringe privately owned rights. Reference herein to any specificcommercial product, or service by trade name, trademark, manufacturer, or otherwise does notnecessarily constitute or imply its endorsement, recommendation, or favoring by the United StatesGovernment or any agency thereof. The views and opinions of authors expressed herein do notnecessarily state or reflect those of the United States Government or any agency thereof.
This report describes research conducted to support the DOE program in indirect coal liquefaction.Specifically, we have studied the attrition behavior of iron Fischer-Tropsch catalysts, their interac-tion with the silica binder and the evolution of iron phases in a synthesis gas conversion process.The results provide signficant insight into factors that should be considered in the design of catalystsfor converting coal based syn-gas into liquid fuels.
Table of Contents page
Executive Summary 2
Technical Objectives 2
Task 1: Catalyst Particulate Synthesis 3
Task 2: Catalyst Binder Interaction 7
Task 3: Catalyst Characterization 9
Figures 1-28 13
This report covers the third six months of this three year grant under the University CoalResearch program. During this period, we have explored the uniaxial compaction method asan approach to derive particle breaking stress. The method was applied to alumina supportgranules obtained from Dr. Robert Gormley at PETC and will be extended to other F-T cata-lysts in future work. We also present ultrasonic fragmentation analysis of Fe/alumina F-Tsamples obtained from PETC. When the particle size evolution is compared with that of thebase UCI catalyst, it is clear that the alumina-supported catalysts show significant improve-ment in particle strength. This work will be continued over the next six month period tobetter quantify the agglomerate strength of F-T catalysts, and to afford comparisons betweenthe uniaxial compaction and ultrasonic fragmentation methods for determining the strengthof F-T catalysts.
During this period, we have continued our study of Fe/silica interactions to provide a funda-mental understanding of the how silica binders influence the activity and attrition resistanceof these catalysts. To understand differences in the reducibility of the iron phase caused bysilica, we have set up a temperature programmed reduction facility. TPR in H2 as well as inCO was performed of Fe/SiO2 catalysts prepared by impregnation as well as by precipita-tion.
We have completed analysis of catalysts received from slurry reactor runs at Texas A&Muniversity (TAMU) and the University of Kentucky Center for Applied Energy Research(CAER) by x-ray diffraction. The analysis results were conveyed to PETC, TAMU and CAERin September 96 are included here for the sake of completeness. The purpose of the XRDanalysis was to determine the phase composition of catalysts derived from a slurry reactionrun using Fe Fischer-Tropsch catalysts. As we describe in this report, the XRD results showthat the carbide phase does not transform into magnetite over the course of a F-T run, both inthe TAMU as well as in the CAER runs. The slow deactivation of these catalysts must then berelated to crystallite growth and loss of active phase surface area. Further work is underwayto corroborate this hypothesis.
The objective of this research project is to perform fundamental research in support of cata-lyst development for slurry phase bubble column reactors for Fischer-Tropsch synthesis. Theoverall program is divided into the following tasks:
Task 1. Catalyst Particulate SynthesisTask 2. Catalyst Binder Interactions.
In task 1, we will first study factors that determine the attrition resistance of slurry phase Fecatalysts. Fundamental understanding of the attrition phenomenon will be used to guide thesynthesis of novel precipitated catalysts that overcome some of the limitations of currentgeneration catalysts. The investigation of catalyst microstructure as a function of treatmentwill help determine the optimal treatment protocols for F-T synthesis catalysts. Since the useof binders is considered essential for providing the desired attrition resistance, the second
task is to perform fundamental studies of catalyst-binder interactions. These studies will usemodel catalysts that can be studied by high resolution transmission microscopy to investi-gate the nature of interfacial phases at the Fe-binder interface. A better understanding of thephenomena that lead to catalyst-binder interactions will help us design improved catalystsfor indirect coal liquefaction.
Task 3. Characterization of catalysts received from CAER, Univ. of Kentucky, and fromTexas A&M.
Task 3 was not included in our original proposal. However, we are pursuing these studies tohelp understand catalyst deactivation under actual reaction conditions.
Technical ProgressTask 1: Catalyst Particulate Synthesis
In the previous six-monthly report we showed how ultrasonic excitation followed by sedigraphparticle size distribution can yield a simple test for the strength of catalyst agglomerates.While the breakdown of particles subjected to ultrasound energy provides a graphic measureof particle strength, a number of assumptions must be made to derive a quantitative measureof particle strength. Hence, during the current six month period we have explored the use ofa more conventional test for particle strength.
Uniaxial Compression Testing
Uniaxial compression testing is a technique for characterizing the strengths of powders andgranular materials. Previously, the conventional method used for compression tests was theBrazilian test, in which individual particles were crushed between two platens (1). Thedrawback to this method was in the variability of strength due to variations of individualparticle sizes and shapes. Furthermore, individual particle fracture loads are small (equiva-lent to a few grams weight) such that the accuracy of the data might not be high.
A simple alternative method consisted of replacing the individual particle with a confinedbed of similar particles, inferring some average individual particle strength parameter fromthe behavior of the whole bed under compression (1). This method is easily achieved using apiston in a cylinder, hence this method involves a uniaxial compaction (as shown on the nextpage).
Confined Uniaxial Compression Test
Uniaxial compression testing has been used by a group at Sandia National Laboratories in thestudy of ceramic granule strength. The tests were performed at the Advanced Materials Labo-ratory (a joint Sandia National Labs- University of New Mexico facility located on the univer-sity research park). For comparison, uniformly sized glass spheres were also used in theirstudy. Diametral compression strength tests, similar to the Brazilian test, were performed(2) and the results were compared with those obtained with the uniaxial compaction test.The uniform-size glass spheres were used to eliminate the effects of shape and size factors,and minimize strength variability. Surprisingly, the results showed that the glass spheres alsoexhibited large variability in strength. The results for ceramic granules and uniform-sizeglass spheres were verified by using Weibull statistics; indeed, results the glass spheres gavesimilar Weibull parameters to those obtained from ceramic granules, indicating a large strengthvariability for individual glass spheres. Although the glass spheres were uniform in size, thelarge variability in strength was thought to arise from the large range in flaw sizes.
To circumvent the tedious task of testing individual granules by the diametral compressiontest, pressure compaction (P-C) tests were also performed by Jill Glass and coworkers at SNL.Compaction behavior of these samples was determined by plotting the relative density of thecompacted sample vs. the log of the compaction pressure as shown on the next page (2).
Granule fracture+ rearrangement
This figure shows how the data of relative density vs log pressure can provide a semi-quanti-tative measure of agglomerate strength. As shown in this plot, compaction data tend to ex-hibit linear regimes that can be attributed to different compaction mechanisms (3). In the firstregime, the gradual increase in relative density is due to particles, such as granules and ag-glomerates, sliding and rearranging without fracture. At this stage little compaction occurs,and only a small percentage of the void space is removed during rearrangement. It is oftenobserved experimentally that this regime has a slope
Click here to load reader